FLUORESCENT SELF-ASSEMBLED POLYPHENYLENE DENDRIMER NANOFIBERSDaojun Liu,† Steven De Feyter,*,† Mircea Cotlet,† Uwe-Martin Wiesler,‡Tanja Weil,‡ Andreas Herrmann,‡ Klaus Mu1 llen,‡ and Frans C. De Schryver*,†Laboratory for Photochemistry and Spectroscopy, Department of Chemistry, Katholieke UniversiteitLeuven (KULeuven), Celestijnenlaan 200F, B-3001 Leuven, Belgium, and Max Planck Institute forPolymer Research, Ackermannweg 10, 55128 Mainz, GermanyReceived June 24, 2003
Introduction Dendrimers have attracted much attention for the past two decades because of their fascinating structure and unique properties such as their globular shape, highly controlled size, radially controlled chemical composition, multivalent periphery, and variable inner volume. Self-assembly of dendrimers with or without guest molecules at the ensemble as well as the single molecule level is of special interest because this creates a wide collection of novel structures and surfaces with higher complexity and promising properties.
A second-generation polyphenylene dendrimer 1 self-assembles into nanofibers on various substrates such as HOPG (Highly ordered pyrolytic graphite) , silicon, glass, and mica from different solvents. The investigation with noncontact atomic force microscopy (NCAFM) and scanning electron microscopy (SEM) shows that the morphology of the dendrimer nanofibers highly depends on substrate, solvent, and preparation method.
Fluorescent nanofibers can be prepared from a polyphenylene dendrimer with chromophores either attached to the periphery of the dendrimer or incorporated in its core.
Fluorescent nanofibers formed from polyphenylene dendrimer 4 with a perylenediimide core show isolated- chromophore emission due to the shielding of the rigid polyphenylene dendrons.
Dendrimer 2 with one perylenemonoimide attached to its periphery self-assembles into fluorescent nanofibers, which exhibit a dimer like emission as a result of the interactions between peripheral chromophores.
Dendrimer 3 with two perylenemonoimides at the rim does not form nanofibers by itself, but mixing of nonfluorescent dendrimer 1 with fluorescent dendrimers 2 or 3 leads to the formation of nanofibers with a homogeneous composition. Therefore, mixing can not only coassemble nonnanofiber- forming dendrimer 3 into nanofibers but also give rise to isolated chromophore emission upon proper dilution.
The self-assembly of dendrimers into mono- or multilayers on a solid substrate through electrostatic interactions, polydentate interactions, or covalent bonding has been investigated. Dendrimers can also self-assemble into three-dimensional nanostructures like blocks in bulk into spherical, cylindrical, and more complex supramolecular an supramacromolecular structures. Polyphenylene dendrimers are a special class of dendrimers, which are characterized by their shape- persistent 3D structures. Polyphenylene dendrimers have been observed to form several hundred nanometer long organized structures when additional alkyl chains are attached to their periphery as well as dendrimer multilayers with gold nanoparticles.
We have recently reported that polyphenylene dendrimers with various cores (such as tetraphenylmethane, biphenyl, and azobenzene) and of different generations can self- assemble into micrometer long nanofibers in addition to the formation of globular dendrimer aggregates, on hydrophobic surfaces such as HOPG and silanized mica. A special case is dendrimer 1 , a second-generation polyphenylene dendrimer containing a tetraphenylmethane core, which exclusively self-assembles into micrometer long nanofibers by drop-casting under controlled atmospheric conditions.
»In this article it was investigated the effect of:»Solvent»Substrate»Atmospheric conditionsOn the formation and morphology of the nanofibers.»And to get insight into the effect of functionalization, itwas investigated:»The self-assembly properties of dendrimers functionalized with one or multiplefluorescent peryleneimide chromophores.»The influence of the number and location of the chromophore(s) within thedendrimer»The effect of mixing with nonfunctionalized dendrimers.
Results and DiscussionSelf-Assembled Polyphenylene Dendrimer 1Nanofibers on Various Substrates. The effect of deposition conditions and substrate properties on the formation of self-assembled structure by dendrimer was examined, of which it was demonstrated the formation of nanofibers under controlled conditions. (A) NCAFM image (25 µm x 25 µm) of dendrimer 1 nanofibers prepared by drop- casting a 1.0 10-5 M dendrimer 1 solution in CHCl3 on a HOPG surface. Dendrimer 1 exclusively self-assembles into fibrillar nanostructures under controlled atmospheric conditions.
(B) A smaller scale NCAFM image (3.5 µm 3.5µm) of a dendrimer 1 nanofiber clusterin part A indicated by a frameIn addition to the formation of discretenanofibers, most of the nanofibers aggregateinto bundles forming clusters (Figure 2B).The length of the nanofibers is typically lessthan 10 micrometers. On a silicon surface, bigger nanofiber clusters composed of nanofibers with a length of tens of micrometers were obtained. The diameter of these clusters ranges from 10 to 200 micrometeres as revealed by AFM and SEM measurements.
The area around the nanofiber cluster in Figure 2C is almost free of dendrimer molecules. Because of the difficulty of preparing a mesoscale flat HOPG surface by cleaving and the presence of numerous steps and kinks over large dimensions, the HOPG surface should be rougher than that of the silicon. This could lead to the formation of smaller and more domains of droplets of dendrimer in solution at the HOPG surface toward the end of the solvent evaporation, which could explain the fact that smaller and more dendrimer nanofiber clusters as well as discrete nanofibers are formed on the surface of HOPG compared to a silicon surface (Figure 2A,C).
(D) SEM image of a dendrimer 1 nanofibercluster on a silicon surface imaged at a tiltedangle of 70°.The ordering of nanofibers into clusters isconsidered to be the result of dewetting.Because of the dewetting in the course of theevaporation process, the dendrime solutionevolves into separated domains, within whichthe nanofibers form and aggregate intoclusters. When THF was used as the solvent, the nanofibers prepared by drop-casting on a silicon surface wer observed to be quite evenly distributed, and they forme a network extending over the entire substrate surface. The rather homogeneous distribution of th nanofibers formed from THF solution on the silicon surface could be ascribed to the improved wetting properties of THF toward the oxidized silicon surface which results in a thin dendrimer solution layer rather than separated domains at the final stage of the solven evaporation.
It was found that the addition of a smallamount o water to the THF atmosphere duringthe drop-castin suppressed the aggregation ofnanofibers.Figures C and D show AFM images of thenanofiber formed from a dendrimer 1 solutionin THF in saturated atmosphere of THF and5% and 10% (v/v) H2O, respectively.In the presence of 10% water, a largenumber of individual curved nanofibers isobtained withmany crossing points (E) A smaller scale NCAFM image of part D. Topography profile along the dotted line indicated in the image is shown beneath. (F) SEM image of part D.
G) NCAFM image (50 µm 50 µm) of dendrimer 1 nanofibers prepared by drop-casting a 2.0 10-6 M dendrimer 1 solution in THF in a saturated environment of THF:H2O ) 80:20 (v/v) on a silicon surface. (J) NCAFM image (10 µm x 10 µm) of dendrimer 1 aggregates prepared byH) A smaller scale NCAFM drop-casting a 2.0 10-6 Mimage of part G. dendrimer 1 solution in THF at a saturated H2O environment on a silicon surface. (I) SEM image of part G.
NCAFM image of dendrimer 1 nanofibers prepared by drop-casting a 2.0 10-6 M dendrimer 1 solution in THF in a saturated environment of THF:H2O 90:10 (v/v) on a glass surface(A, 25 µm x 25 µm) and on a mica surface (B, 30 µm 30 µm).Self-Assembly of Mixtures of Dendrimers. NCAFM image (A, 30 µm x 30 µm), confocal fluorescence image (B, 40 µm x 40 µm), and the emission spectrum (C) of dendrimer 2 nanofibers;
NCAFM image (D, 50 µm 50 µm), confocal fluorescence image (E, 40 µm 40 µm), and the emission spectrum (F) of dendrimers 1 and 2 mixed (molar ratio, 5:5) nanofibers NCAFM image (G, 50 µm 50 µm), confocal fluorescence image (H, 40 µm 40 µm), and the emission spectrum (I) of dendrimers 1 and 2 mixed (molar ratio, 9:1) nanofibers.All nanofibers are prepared by drop-casting a 2.0 10-6 M (total concentration) dendrimer solution in THF on asilicon surface in a saturated environment of THF:H2O ) 90:10 (v/v). The emission spectrum (excitation wavelength488 nm) of dendrimer 1 in THF is shown as a dotted line in (C).
NCAFM image (A, 20 µm 20 µm), confocal fluorescent image (50 µm 50 µm), andthe emission spectrum (C) of nanofibers prepared by drop-casting a 1.0 10-5 Mdendrimer 4 solution in CHCl3 on a HOPG surface in a saturated CHCl3atmosphere. The emission spectrum of dendrimer solution in CHCl3 is shown as adotted line in (C).
NCAFM image (A, 20 µm 20 µm), confocal fluorescence image (B, 40 µm 40 µm), and the emission spectrum (C) of dendrimer 3 nanoaggregatesNCAFM image (D, 50 µm 50 µm), confocal fluorescence image (E, 40 µm 40 µm),and the emission spectrum (F) of dendrimers 1 and 3 mixed (molar ratio, 5:5)nanofibers
NCAFM image (G, 50 µm 50 µm), confocal fluorescence image (H, 40 µm 40 µm), and the emission spectrum (I) of dendrimers 1 and 3 mixed (molar ratio, 9:1) nanofibers.All nanofibers are prepared by drop-casting a 2.0 10-6 M (total concentration) dendrimersolution in THF in a saturated environment of THF:H2O ) 90:10 (v/v) on a silicon surface.
Conclusions.Polyphenylene dendrimer 1 in different organic solvents exclusively self-assembles into nanofibers on various substrates upon drop-casting under asaturated solvent atmosphere.While nanofiber clusters are formed on a HOPG and silicon surface from itssolution in CHCl3, dendrimer 1 self-assembles into a nanofiber network from asolution in THF on a silicon, glass, or mica surface, which distributes over thewhole surface of the substrate.Addition of a small amount of water to the drop-casting THF atmospheresuppresses the nanofiber aggregation and gives rise to individual nanofibers. Ithas been demonstrated that the morphologies of the dendrimer 1 nanofibers canbe regulated by changing solvent, substrate, and preparation method.
»Fluorescent nanofibers can be prepared from a polyphenylene dendrimer with afluorescent functional group either attached to its periphery or incorporated in itscore.»Polyphenylene dendrimer 2 with a perylenemonoimide chromophore attached tothe periphery exclusively self-assembles into fluorescent nanofibers, which showsdimer-like emission.»Polyphenylene dendrimer 4 with a perylenediimide core also self-assembles intofluorescent fibers, but the dendrimer arms shield the perylenediimide core.»Mixtures of nonfluorescent dendrimer 1 and fluorescent dendrimers 2 or 3 lead tothe exclusive formation of fluorescent nanofibers.»The emission spectrum of these nanofibers changes upon decreasing the relativeconcentration ratio of the fluorescent chromophore, indicating that the fluorescentdendrimers are homogeneously distributed within the nanofibers.»Moreover, the nonfluorescent dendrimer 1 can act as a guest to coassembleotherwise non-fiberforming dendrimers into micrometer long nanofibers.
A tetramer model of dendrimer 1 built by the MMFF method.
A particular slide catching your eye?
Clipping is a handy way to collect important slides you want to go back to later.